Acta melall. Vol. 37, No. 5, pp. 1415-1420, 1989 Printed in Great Britain
OOOI-6160189$3.00 + 0.00 Pergamon Press plc
EFFECT OF TEMPERATURE ON THE DENSIFTCATION/CREEP VISCOSITY DURING SINTERING MAY-YING CHU and L. C. DE JONGHE Lawrence Berkeley Laboratory, Materials and Chemical Sciences Division and Department of Materials Science and Mineral Engineering, University of California. Berkeley, CA 94720. U.S.A.
M. N. RAHAMAN University of Missouri-Rolla
Ceramic Engineering Department, (Received
Rolla, MO 65401, U.S.A.
Abstract-The densification and creep rates of polycrystalline zinc oxide and of alumina powder compacts have been measured simultaneously in a loading dilatometer, under constant heating rate and constant temperature conditions. The data show that the ratio of the densitication to the creep rate is remarkably constant within a wide temperature range for densification, from the earliest stages of densification to at least the onset of the final stage. As a consequence, the ratio of the densi~cation to the creep viscosity is nearly independent of temperature or sintered density. The analysis leads to a simple method for determining the simultaneous densification over the creep rate ratio. The implications of the result for the processing of heterogeneous ceramics and composites are discussed. RBsumGLes vitesses de densification et de fluage de l’oxyde de zinc polycristallin, et de poudres d’alumine compactees ont it& mesurees simultanement dans un dilatomitre de charge, dans des conditions de vitesse de chauffage et de temptrature constantes. Le rapport densification~vitesse de &age est remarquablement constant dans un vaste domaine de temperatures pour la densi~~tion, depuis les premiers stades de ta densification jusqu’au debut du dernier stade au moins. 11en resulte que ie rapport densification/viscosite de fluage est a peu pres independant de la temperature ou de la densiti apres frittage. A partir de cette analyse, nous proposons une mtthode simple pour determiner le rapport de la densification a la vitesse de fluage. Nous discutons les consequences du rtsultat dans le domaine de l’blaboration de ceramiques hettrogenes et de composites. Z~~menf~~g-Die Verdichtun~- und Kriechraten von polykristallinem Zinkoxid und von Aluminiumoxid-Pulve~re~lingen wurden gleichzeitig in einem Lastdifatometer unter konstanter ErwHrmung und unter konstanten Temperaturbedingungen gemessen. Die Ergebnisse zeigen, da13das VerhLltnis zwischen der Verdichtungs- und der Kriechrate in einem weiten Temperaturbereich der Verdichtung bemerkenswert konstant ist. Dieser Bereich reicht vom friihesten Einsatz der Verdichtung bis mindestens zum Einsatz des Endstadiums. Folglich ist das Verhiiltnis zwischen der Verdichtung und der Kriechviskositiit nahezu unabhangig von der Temperatur oder der Sinterdichte. Die Analyse fiihrt zu einer einfachen Methode, die gleichzeitige Verdichtung iiber dieses Verhihnis zu messen. Die Bedeutung des Ergebnisses fur die HersteI~ung heterogener Keramiken und Verbundwerksto~e wird diskutiert.
1. INTRODUCTION It is widely recognized that the densification behavior of powder compacts depends significantly on their uniformity, and efforts to achieve a high degree of uniformity in the initial structure of powder compacts have been very fruitful. In many if not most practical powders, however, agglomerate formation cannot be completely avoided. Further, in a number of important cases, such as the particulate composites, inhomogeneities are an essential part of the system. The presence of heterogeneities in the powder compacts lead to local, non-uniform densification rates which, in turn, produce stresses in the surrounding matrix that oppose densiflcation. Unless these stresses are relieved by shear deformation (i.e. creep) they can lead to a significant reduction in densification rates and may exacerbate the develop-
ment of deleterious crack-like voids around inclusions [l-9]. In addition, clustering of the dispersed phase will lead to the formation of extended skeletal segments of the inert particles, arresting macroscopic densification, as was discussed by Lange [lo]. These clustering effects, rather than the back-stresses generated by local densification rate mismatch, are likely to dominate the dens&cation behavior at high inclusion content in particulate composites. If techniques were employed that prevented the fo~ation of percolation networks of the inert phase, then the backstresses resulting from local densification rate mismatch would remain as the most significant factor impeding free sintering of particulate composite powder compacts. It has been shown by De Jonghe et‘al. 151and by Scherer et al. [I I] that the backstresses arising during
CHU ef al.:
the densification of particulate composite powders are simply viscous, i.e. proportional the instantaneous densification rate of the matrix. This leads to a matrix densification rate that is determined by the volume fraction of the dispersed inert phase and by the ratio of the creep viscosity over the densification viscosity i, = ~,o/]l + 4(rl&Y-/(l
where the superscript dot represents differentiation with respect to time, and where i, = densification rate of the matrix for the composite i,, = matrix densification rate at f = 0 f = volume fraction of the hard inclusion qc = creep viscosity of matrix qd = densification viscosity of the matrix defined by where (C/G) is the sintering GllO . = [email protected]
@h~ stress [S]. The magnitude of the ratio of the creep viscosity over the densification viscosity of the matrix is therefore an important parameter in the densification of particulate systems in which the inclusion phase is uniformly distributed, even though it is unlikely to vary by orders of magnitude, as first postulated [2, 31. Practically, densification cannot be carried out isothermally, and it is well known that significant densification usually occurs by the time the isothermal sintering condition has been reached. Alternatively, non-isothermal processing methods might be considered to affect the microstructural evolution of the powder compact. Thus, the dependence of the ratio of the densification rate over the creep rate on temperature needs to be examined for non-isothermal conditions. From the ratio of the densification rate over the creep rate, the ratio of the creep viscosity over the densification viscosity may be inferred, allowing an assessment of the possible effects of heating schedules on densification of particulate composites. Rahaman and De Jonghe have used the technique of loading dilatometry  to measure simultaneously the densification and creep rates in a number of ceramic powder systems [13-191. Generally, for each system, the densification and creep rates were measured at a single, isothermal sintering temperature. A selection of the data is shown in Fig. 1, where the ratio of the linear densification rate to the creep rate is plotted as a function of relative density. Over a wide density range, covering at least the intermediate stage of sintering, the ratio of the densification over the creep rate is almost independent of density. The value of this ratio decreases with decreasing green density and is system specific. In a study on the creep-sintering of soda-lime glass powder compacts  conducted at two closely separated temperatures ($0 and 605°C) the data indicated that the ratio of the densification to the tReagent grade, Mallinckrodt Inc., Paris, Ky. IAlcoa Chemicals, Pittsburg, Pa.
creep rate was nearly independent of temperature (Fig. 1). The objective of the present paper is to examine the dependence of the densification and creep rates on temperature from experiments conducted over a wide temperature range for a constant heating-rate schedule. Data were obtained for two different crystalline powders: ZnO and Al,O,. For comparison, data were also obtained on the isothermal creep-sintering of alumina.
2.1. ZnO Zinc oxide? powder compacts (6mm in diameter by 6 mm) having a green density of 0.44 + 0.01 of theoretical were made by uniaxial compaction in a tungsten carbide die at x 10 MPa. The same powder was used by the present authors in earlier sintering studies [7, 131. The compacts were sintered in air in a loading dilatometer , under uniaxial loads of 0 or 7 N, at a constant heating rate of 4”C/min. The experiment was stopped at lOOO”C, where densification was nearly complete. The load of 7 N, corresponding to an initial stress on the green compact of 0.24 MPa, was applied when the temperature had reached 500°C when shrinkage just commenced. The mass and dimensions of the samples were measured before and after sintering and the final densities were verified using Archimedes’ method. In a separate set of experiments, sintering under the load of 7 N was terminated at temperatures between 500 and lOOO”C, and the dimensions of these compacts were measured using a micrometer. 2.2. Aimina Procedures similar to those for ZnO were used for the alumina powder.f The powders were compacted 1.2 Z”O
0 3 6
9 YEsan C”,
._:: !e z 0 s
Fig. 1. Ratio of the densification strain rate to the creep strain rate vs relative density at a constant applied stress of 0.2 MPa. The numbers in parenthesis represent the relative green density and the sintering temperature (“C).
in a die to a green density of 0.52 + 0.01 of theoretical. They were then sintered in air at constant heating rate, up to a maximum temperature of 1400°C. The loads of 0 and 7 N were applied from 1000°C on, at which point densification could not yet be detected. In addition to constant heating rate experiments, samples were isothermally sintered at 135O‘C in air, for 2 h. under a load of 7 N. These samples were inserted rapidly into the hot zone of the dilatometer and reached the sintering temperature in about 557 min. After the initial temperature transient the load was applied.
0.4 fJ,= 0.24
' 1, 0.1.
fJ,= 0 HP3 /
,i:/' I/ / '/ 1, //
Fig. 3. Axial strain
3.1. ZnO Figure 2 shows the results for the axial true strain, t,, vs temperature for the ZnO samples sintered at a constant heating rate of 4”C/min under zero applied stress and under an initial stress of 0.24 MPa. Each curve is the average of two runs under the same conditions and each is reproducible to f 1%. The results for the axial true strain, c,, vs the radial strain, c,, determined by terminating the sintering runs at temperatures between 500 and 1000-C, are shown in Fig. 3; each data point was obtained using a different sample. The shrinkage of the sample sintered under zero stress is seen to be almost isotropic. Within the limits of experimental error, the applied stress caused no change in the density; the final density of the sample sintered under the initial stress of 0.24 MPa was 0.97 compared with 0.96 for the sample sintered under zero stress. The deformation of the sample under the action of the applied stress was therefore constant volume creep.
ments, while line B corresponds to the isothermal experiments, both at an applied load of 7 N. Line B does not go through the origin, since some shrinkage has already occurred in the heat-up period, before isothermal conditions were reached and the load was applied. Line C corresponds to the zero load sintering.
In this section the densification strain rate, i,, and the creep rate, i,, are related to the axial strain/radial strain plot, t, vs c,. From the analysis, some simplified experimental procedures emerge. For a body loaded uniaxially and deforming uniformly it is readily shown that the linear densification strain is 36, = f, + 26, while at the same time, for the total axial strain,
3.2. Alumzint, Figure 4 shows the axial true strain, czr vs the radial true strain, t,, for the alumina powder compacts. Line A corresponds to the constant heating rate experi-
c, = c, + t* from which t, = 2(t, - cc)/3
0.08 - G 0.06
Fig. 2. Axial strain vs temperature for ZnO powder compacts sintered at a constant heating rate of 4”C/min and under the uniaxial stresses shown.
Fig. 4. Axial strain vs radial strain for A&O,. (A) Heating rate, 4”C/min; applied load, 7 N, (B) isothermal, 1350°C; applied load, 7 N. and (C) heating rate. 4“Cimin; applied load, 0 N.
At fixed density, i.e. p = 0, constant requires that
cc= -26 IC
Fig. 5. Various
in a densifying and creeping compact.
where the meaning of the various strains is indicated in Fig. 5. If the creep rate at constant uniaxial stress is linearly proportional to the densification rate then one must expect that c,= kc,.
The relative densification and creep strains as shown in Fig. 6 can be obtained from dilatometer data in Figs 2 and 3, and density measurements. The procedure is particularly simple in the case of constant volume deformation, as was the case here. The densification strain rate, fi/3p, and the creep strain rate, C,, can be obtained as a function of temperature by fitting smooth curves through the data of Fig. 6 and differentiating according to equations (6) and (7) p/3p = i, = (4/p) dp /dT i, = 4 dc,/dT.
where t,, is the radial component of the creep strain. The locus of cz at some fixed density in a plot of t, vs cr is then a straight line with a slope of - 1:2, as shown in Fig. 7(a). The data for constant load creep should then follow a straight line in the c,/E, plot and intersect a constant density line when the sintered density with applied uniaxial stress equals that of the sintered density at zero load. This intersection for ZnO is shown in Fig. 7(a), and shows at once that creep indeed occurs at nearly constant volume. Similar results are obtained for A1,03. Near constant volume creep has been observed for all ceramics studied so far by low-load loading dilatometry. It is then possible, with considerable confidence, to identify the t, value corresponding to a measured shrinkage strain, t,, for a particular density, by making a construction as shown in Fig. 7(b), without the need of measuring t, directly. As seen from equation (8), the ratio of i,/i, is very sensitive to variations in the values of k. In the actual 0.4 (a)
T is the temperature,
and the factor 4 arises from the constant heating rate of 4°C per minute that was used in the experiments when time is expressed in minutes. Equations (4) and (5) are also valid as strain rate equations so that id/it = (k + 2)/2(k - 1).
Fig. 6. Relative density, p. and creep strain, E,, calculated from Figs 2 and 3 and equations (6) and (7).
Fig. 7. (a) Axial strain vs radial strain for ZnO with constant density line. (b) Hypothetical construction of the axial strain versus radial strain from t, (measured from sample), isotropic line, and constant density line.
CHU et al.:
experiment, the data are collected at constant load rather than at constant stress. Since the sample cross sectional area, A, changes from the initial one, A,, as a result of densification and creep, the applied stress, rr, differs from the initial stress, ~7~ (T = a,, A,/A
An estimate can be made readily of how much change in k would be associated with the changing stress for the experimental conditions adopted here, or what the error would be if the constant load experiment is simply treated as if it were at constant stress. To allow for this estimate the total strains are needed, and for the sake of illustration a simple creep and densification relationship, which materials such as ZnO obey well for a large part of the densification, may be adopted -td
and -CC = B,cr/t = B,q,(A,/A)t where B, and B, are kinetic constants. time one has A,,/A = (R,/R)’
(12) At the same
when R, and R are the initial and the instantaneous radius of the sample cross section. To a first approximation the creep rate may be expressed as -i,
At low loads, the creep strain can be taken to be much smaller than the densification strain (typically t, < 0.2 cd). Then, with t, z cd, integration yields t,(t, a) = t,(t, a,)(1 -Q).
Equation (15) can be used to correct k to constant stress. The necessary information is shown in Fig. 8 where line 1 is the constant load line, line 2 is the isotropic line and line 3 is the constant density line. The correction to each t, and t, datum point for ZnO is shown in Fig. 9.
uncorrected d, /P corrected ‘1 , ,, /
1, ,’ N / N /
Fig. 9. Axial strain vs radial strain for ZnO. Constant load at 7 N (uncorrected), constant stress at 0.24 MPa (corrected), 0 load (isotropic). The values of k that follow from such an analysis are 1.33 for ZnO, and 1.29 and 1.30 for A&O, done under constant heating rate and isothermal conditions respectively. Using equation (8) this would then yield values of the densification rate over the creep rate as 5.00 for ZnO, and 5.67 and 5.50 for Al,O, all at a stress of 0.24 MPa. More accurate data can be obtained from the creep rate (converted to constant stress rates by compensating for the crosssectional area change) and densification rate measurments, rather than from the total strain determination. The ratios of i,/i, obtained from the rate measurements are 4.5-5.0 for ZnO and 5.7-6.5 for Al,03. The data for ZnO is shown in Fig. 10. The two methods for obtaining i, /CCare in close agreement. This shows the total strain determination is useful for generating values of i,/i, with minimum experimentation. 5. DISCUSSION
Figure 10 shows the ratio of the densification rate over the creep rate for ZnO. This ratio is nearly constant as a function of temperature. for the
5.0 - ( cl ) 4.5 > 2 4.0-
Fig. 8. Corrections of axial and radial strain from constant load (f,, c~) to constant stress (t;, t;).
Fig. 10. (a) Ratio of the densification to the creep strain rate vs temperature for the uniaxial stress shown. (b) Relative densification rate, p/p, and creep strain rate, i,, vs temperature at the constant uniaxial stress shown.
CHU et al.: DENSIFICATION/CREEP VISCOSITY DURING SINTERING
ceramics examined here: ZnO and Al,03. The results of the isothermal loading dilatometry in Fig. 1 demonstrate that the creep rate over the constantstress densification rate is also insensitive to density changes for a particular system. In addition, as seen in the AllO3 experiments, densification rate over the creep rate is equal in this experimental case for both the isothermal condition and the constant heating rate condition. Therefore, the densification over the creep rate may be obtained reliably from a nonisothermal experiment, extending the measurement range to the earliest stages of densification. Deviations of the proportionality between the constant stress creep rate and the simultaneous densification rate would be manifested by the i, vs i, data not extrapolating through the origin. Such a deviation is not apparent in Figs 4 and 9; thus i,/i, is nearly constant from the onset of sintering. The last stages of densification remain unexplored to date, since accurate measurements become difficult at high densities. The near-constancy of the densification rate over the creep rate under widely varying conditions of temperature and density are perhaps somewhat unexpected, and indicate at the same time that relatively little benefit is to be expected from non-isothermal densification schemes for particulate composites. The benefits that may result from non-isothermal heating schedules would, in fact, be those that are obtained in the improved sintering behavior or microstructure of the inclusion-free matrix. The ratio of the creep viscosity over the densification viscosity does not follow directly from the measured values of the densification rate over the creep rate. To obtain these values from loading dilatometry experiments, it will be necessary to measure precisely the small density increases that result from the hydrostatic component of the applied uniaxial stress. In principle, this should be possible, since the hydrostatic component of the applied stress, ga, can be added simply to the sintering stress, Z/Q i,(a,) = [([email protected]
) + tJ31h
= &(a, = 0) + cJ31,
so that with i, = a&l,
one obtains ?,/Vrd=3[id(~a)-id(ba=O)llic.
The measurements presented here were not sufficiently accurate to determine whether this ratio is indeed constant throughout the densification process. In one liquid phase sintering system, accurate measurements showed that the ratio was indeed constant throughout the intermediate stage of densification and approximately equal to 2. Theoretical consideration of Scherer also lead to the conclusion that the ratio of the creep viscosity over the densification viscosity should be nearly constant and equal to 2. Further, the constancy of the densification rate over
the creep rate would require some unlikely compensation mechanisms to be at work if the viscosity ratio were not constant. All these considerations lead to the conclusion that both the sintering stress, z/Q, and the creep viscosity over the densification viscosity, n,/nd, are constant from the very early stages to late into the intermediate sintering stage. 6. CONCLUSIONS The results of the present study show that, when constant volume creep deformation occurs during sintering, the ratio of the densification to the creep rate is almost independent of temperature. Within the useful temperature range for densification, the ratio of the densification to the creep viscosity is nearly independent of temperature. The present data have important implications for the sintering of heterogeneous ceramics and composites. The matrix densification rate of a particulate composite containing a fixed volume fraction of inclusions is predicted to be inversely proportional to its creep (or densification) viscosity. Acknowledgements-This work was supported by the Division of Materials Sciences, Office of Basic Energy Sciences, U.S. Department of Energy, under Contract No. DE-AC03-76SF00098. This work was oerformed in the Lawrence Berkeley Laboratory when Dr*M. N. Rahaman was Visiting Staff Scientist in the Materials and Chemical Sciences Division.
REFERENCES 1. A. G. Evans, J. Am. Cerum. Sot. 65, 497 (1982). 2. R. Raj and R. K. Bordia, Actu mefall. 32, 1003 (1984). 3, C. H. Hsueh, A. G. Evans, R. M. Cannon and R. J. Brook, Acfa metall. 34, 927 (1986). 4. C. H. Hsueh, A. G. Evans and R. M. McMeeking, J. Am. Ceram. Sot. 69. C6&C66 (1986). 5. L. C. De Jonghe and M. N. Rahaman, ictn metall. 36, 223 (1988). 6. G. W. Scherer, J. Am. Cerum. Sot. 70, 719 (1987). 7. L. C. De Jonghe, M. N. Rahaman and C. H. Hsueh, Acta metall. 34, 1467 (1986). 8. M. N. Rahaman and L. C. De Jonghe, J. Am. Ceram. Sot. 70, C348-C351 (1987). 9. M. N. Rahaman and L. C. De Jonghe, in Proceedings of the First International Conference on Ceramic Powder Processing Science (edited by G. L. Messing, E. R. Fuller and H. Hausner) (1988). In press. 10. F. F. Lange, J. Metr. Resd., 2, 59 i1987). 11. G. Scherer and R. Bordia. Acta metall. To be nublished. 12. L. C. De Jonghe and M. N. Rahaman, *Rev. Sci. Instrum. 55, 2007 (1984). 13. M. N. Rahaman and L. C. De Jonghe, J. Mater. Sci. (1988). In press. 14. M. N. Rahaman and L. C. De Jonghe, J. Am Cerum. Sot. 67, C205-C207 (1984). 15. M. N. Rahaman, L. C. De Jonghe and R. J. Brook, J. Am. Ceram. Sot. 69, 53 (1986). 16. M. Lin, M. N. Rahaman and L. C. De Jonghe, J. Am. Cerum. Sot. 70, 360 (1987). 17. L. C. De Jonghe and S. Srikanth, J. Am. Ceram. Sot. To be published. 18. M. N. Rahaman, L. C. De Jonghe, G. W. Scherer and R. J. Brook, J. Am. Ceram. Sot. 70, 766 (1987). 19. M. N. Rahaman, L. C. De Jonghe and M-Y. Chu, J. Am. Ceram. Sot. To be published.